# MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER MODIFIED ... ?· MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER…

Post on 08-Sep-2018

212 views

Embed Size (px)

TRANSCRIPT

MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER MODIFIED ASPHALTIC CONCRETE TXDOT DESIGNATION: TEX-232-F

CONSTRUCTION DIVISION 1 10 EFFECTIVE DATE: AUGUST 1999

Test Procedure for

MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER MODIFIED ASPHALTIC CONCRETE

TxDOT Designation: Tex-232-F Effective Date: August 1999

1. SCOPE

1.1 Use this procedure to determine the proper proportions of approved aggregates and rubber-asphalt blend which, when combined, will produce a mixture that will satisfy the specification requirements. Typical examples for design are provided.

1.2 The values given in parentheses (if provided) are not standard and may not be exact mathematical conversions. Use each system of units separately. Combining values from the two systems may result in nonconformance with the standard.

2. DEFINITIONS

2.1 Bindera blend of asphalt and ground rubber.

3. APPARATUS

3.1 Apparatus listed in the following test methods:

Tex-200-F

Tex-201-F

Tex-202-F

Tex-205-F

Tex-206-F

Tex-207-F

Tex-227-F.

MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER MODIFIED ASPHALTIC CONCRETE TXDOT DESIGNATION: TEX-232-F

CONSTRUCTION DIVISION 2 10 EFFECTIVE DATE: AUGUST 1999

PART IDETERMINING OPTIMUM GRADATION

4. PROCEDURE

4.1 Obtain representative samples of each processed aggregate proposed for use in accordance with Tex-221-F. Approximately 45 kg (100 lb.) of each aggregate stockpile will be required.

4.2 Dry the aggregate in an oven at a temperature between 38 and 150C (100 and 302F).

4.3 Obtain the average gradation of each proposed aggregate stockpile in accordance with Tex-200-F, Part II. Use samples taken from several locations in the stockpile and average the results. When this is not possible, quarter aggregate samples received in the laboratory to use for the sieve analysis.

4.4 Determine the 24-hour water absorption and specific gravity of each size of each aggregate in accordance with Tex-201-F and Tex-202-F. Note 1Normally, specific gravities are not determined for size fractions consisting of less than 15% of the individual aggregate. Assign smaller size fractions of the water absorption and specific gravity of the next adjacent size fraction for which values were determined.

4.5 Calculate the initial desired combined gradation from the gradations of the stockpiles proposed for use.

4.5.1 As a guideline, keep a ratio of 1.52.0 between the two coarsest sieves on which aggregate is retained. Use this initial gradation only to determine aggregate grading factors.

4.5.2 In Table 1 the initial gradation has a coarse to fine aggregate ratio of 80/20 and a 1.67 ratio between the two coarsest sieves.

4.6 Prepare 5000 g batches with 4.0% asphalt for each of the coarse-to-fine aggregate ratios. (See Section 5.) Follow Tex-205-F.

4.7 Mold three samples of mix from each of the batches in accordance with Tex-206-F.

4.8 Determine the bulk specific gravity of each of the compacted specimens in accordance with Tex-207-F.

4.9 Determine the theoretical maximum specific gravity of each of the batches in accordance with Tex-227-F.

4.10 Calculate the density of each of the molded specimens in accordance with Tex-207-F.

4.11 Plot the average volumetric proportion of total retained on the 2.00 mm (No. 10) sieve for each set of molded specimens versus their average density. (See Figure 1.)

4.12 Pick the point that gives the maximum density on the curve in Figure 1.

MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER MODIFIED ASPHALTIC CONCRETE TXDOT DESIGNATION: TEX-232-F

CONSTRUCTION DIVISION 3 10 EFFECTIVE DATE: AUGUST 1999

4.12.1 Draw a line from the peak down to where it intersects the x-axis and read the total volume of + 2.00 mm (No. 10). (See example in Figure 1.)

4.12.2 The optimum density occurs at a density of 97.3% and a volume of 66.0% retained on the 2.00 mm (No. 10) sieve.

4.13 Add 2.5% to the total volume retained on the 2.00 mm (No. 10) sieve. This value will be the new target used in Part II. (See example in Figure 1.) The new target gradation will be 68.5% by volume retained on the 2.00 mm (No. 10) sieve.

Figure 1Density vs. Volume + No. 10

5. CALCULATIONS

5.1 Determine grading factors for coarse aggregate:

Grading factorindividual retained on each sieve

total retained on mm No sieve

%% . ( . )2 00 10

5.1.1 Example from Table 1:

5.1.1.1 The amount passing the 9.5 mm (3/8 in.) and retained on 4.75 mm (No. 4) sieve = 50%. The total retained on the 2.00 mm (No. 10) sieve = 80%.

5.1.1.2 The grading factor = 50/80 = 0.625 for the 9.5 mm - 4.75 mm (3/8 in.- 4.75 mm (No. 4)) fraction.

MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER MODIFIED ASPHALTIC CONCRETE TXDOT DESIGNATION: TEX-232-F

CONSTRUCTION DIVISION 4 10 EFFECTIVE DATE: AUGUST 1999

5.2 Determine grading factors for fine aggregate:

Grading factorindividual retained on each sieve

total pas g mm No

%

% sin . ( . ) .2 00 10 6 0%

5.2.1 Example from Table 1:

5.2.2 The amount passing the 2.00 mm (No. 10) sieve and retained on the 425 m (No. 40) sieve = 10% and the total % passing the 2.00 mm (No. 10) sieve = 20%.

5.2.3 The grading factor = 10/(20-6) = 0.714 for the 2.00 mm- 425 m (No.10-no. 40) size fraction.

5.3 Calculate combined gradations for coarse-to-fine aggregate ratios of 60/40, 65/35, 70/30, 75/25, 80/20, and 85/15. Use the grading factors determined in Sections 4.2 and 4.3 to keep the same aggregate proportions.

5.3.1 Example from Table 1:

5.3.1.1 For a coarse-to-fine aggregate ratio of 60/40, the % passing the 9.5 mm (3/8 in.) sieve and retained on the 4.75 mm (No. 4) sieve will be (0.625)(60%) = 37.5%. The % passing the 2.00 mm (No. 10) and retained on the 425 m (No. 40) will be (.714)(34%) = 24.2%.

5.4 Calculate volume of total retained on the 2.00 mm (No. 10) sieve for each set of molded specimens:

% ( / ). ( . ) . ( . )V V V xmm No mm No s2 00 10 2 00 10 100

Where: V2.00 mm (+10) =W2.00 mm (+No. 10) / G2.00 mm (+No. 10) = Volume of aggregate retained on 2.00 mm

(No. 10) sieve Vs = Volume of molded specimen = Ws/Gs Ws = Weight of dry molded specimen, Tex-207-F War = Weight of binder in molded specimen W-2.00 mm (-10) = Weight of aggregate passing 2.00 mm (No. 10) sieve W2.00 (+10) = Weight of aggregate retained on 2.00 mm (No. 10) sieve Vair = Volume of air Var = Volume of binder = War/Gar VMA = Vair + Var V-2.00 mm (-10) = W-2.00 mm (-No. 10)/G-2.00 mm (-No. 10) = Volume of aggregate passing 2.00 mm (No.

10) sieve Gs = Bulk specific gravity of molded specimen, Tex-207-F G2.00 mm (+10) = Bulk specific gravity of aggregate retained on 2.00 mm (No. 10) sieve,

Tex-201-F

MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER MODIFIED ASPHALTIC CONCRETE TXDOT DESIGNATION: TEX-232-F

CONSTRUCTION DIVISION 5 10 EFFECTIVE DATE: AUGUST 1999

G-2.00 mm (-10) = Specific gravity of aggregate passing 2.00 mm (No. 10) sieve, Tex-201-F and Tex-202-F

Gar = Specific gravity of binder at 20C (68F).

5.5 Figure 2 shows a graphical representation of components of a molded specimen.

Figure 2Volumetric Analysis of Molded Specimens.

Note 2The sum of the volumetric proportions (V2.00 mm (+No. 10) + V-2.00 mm (-No. 10) + Var + Vair) may not total 100%, caused by errors in determining aggregate specific gravity. Check errors greater than 3%.

Table 1Trial Gradations

Sieve Size Initial Gradation

Grading Factor % Retained on 2.00 mm (No. 10)/% Passing 2.00 mm (No. 10)

60/40 65/35 70/30 75/25 80/20 85/15

12.59.5 mm (1/23/8 in.) 0

9.54.75 mm (3/8 in.4.75 mm [No.4])

50.0 50/80 = 0.625 37.5 40.6 43.8 46.9 50.0 53.1

4.752.00 mm (No. 410) 30.0 30/80 = 0.375 22.5 24.4 26.3 28.1 30.0 31.9

2.00 mm425m (No. 1040)

10.0 10/(20 - 6) =0.714 24.2 20.8 17.1 13.6 10.0 6.4

425180 m (No. 4080) 2.0 2/(20 - 6) = 0.143 4.9 4.1 3.4 2.7 2.0 1.3

180 m (No. 80)No. 200 2.0 2/(20 - 6) = 0.143 4.9 4.1 3.4 2.7 2.0 1.3

Pass No. 200 6.0 N/A 6.0 6.0 6.0 6.0 6.0 6.0

TOTAL 100.0 100.0 100.0 100.0 100.0 100.0 100.0

MIXTURE DESIGN PROCEDURE FOR CRUMB RUBBER MODIFIED ASPHALTIC CONCRETE TXDOT DESIGNATION: TEX-232-F

CONSTRUCTION DIVISION 6 10 EFFECTIVE DATE: AUGUST 1999

PART IIDETERMINING OPTIMUM ASPHALT CONTENT

6. PROCEDURE

6.1 Weigh enough aggregate, asphalt, and crumb rubber to make a 5000 g batch of mix using the stockpile percentages in Section 7.5. Use the binder content determined in Table 2.

6.2 Heat the aggregate to a minimum temperature of 190C (375F).

6.3 Heat the asphalt and crumb rubber to 190C (375F).

6.4 Blend thoroughly and place in the 190C (375F) oven for approximately 30 minutes.

6.5 Stir thoroughly and leave the blend for another 30 minutes at the same temperature.

6.6 Remove from the oven at the end of 1 hour and measure the viscosity using a Haake viscometer.

6.6.1 If the viscosity meets the required specification, proceed to Section 6.7.

6.6.2 If the viscosity is below the minimum requirement, stir the binder thoroughly and return it to the 190C (375F) oven for 30-minute increments until it reaches a satisfactory viscosity.

6.7 Thoroughly stir the heated binder and add the appropriate amount to the heated aggregate.

6.8 Mix with a mechanical mixer in accordance with Tex-205-F.

6.9 Weigh three separate 1000 g samples of the mix for molding. Save the remaining mix for determining the theoretical maximum specific gravity.

6.10 Cure all four samples in an oven

Recommended